Porter easterling phase transformations in metals and alloys 2th ed
Published by C h a p a n L Hall, 2-6 Bormdary Row,London SEl m,LXChapman & Hall, 2-6 Boundary Raw, London SEl 8HN, UK Chapman & Eldl GmbH, Pappclallee 3, 69469 Wtinbeim, Germany ContentsChapman &Hall USA, 115 fifth P:*ermt, NEWYO&, NY 10003, USAChaimao Bt HaU Japan, l7?-Japan, Kyowa Building, 3F, 2-2-1 Ruahwachu,Chiyoda-b, Tokyo 102, JapanChapman &Hall Australia, 1M Dodds Stnet, South Mtlboumc, Victoria 3205, Preface to the second edition xiAustralia Preface to rhe first edition xiiChapman & Hall India, R. Seshadri, 32 Stcond Main Road, CIT East, Madnrs600 035, India I Thermodynamia and Phase Diagrams 1.1 EquilibriumFirst edition 1981 1.2 Single ~ o r n ~ o n e n f SystemsReprinted 1982, 1983, 1984, 1986, 1987, 1988, 1989, 1990, 1992 1.3.1 Gibhs Free Energy as a Function of TemperatureSecond edition 1992Reprinted I993 (twice), 1995, 1996 1.1.1 Pressure Effects 1.2.3 The Driving Force for Soliditicatiun 1.3 Binary Solutions0 1981, I992 D.A.Porter and K.E.Easterling 1.3.1 The Gibbs Free Enerpy of Binary SolutionsTypeset in 10112pt Times by Bed-set Typcseuw hd,Rong Kong , 1.3.2 Ideal SolutionsPrinted in Gnat Brimin by T.J.Pms (jadstow) Ltd, Cornwall 1.3.3 Chemical Potential 1.3.4 Regular SolutionsISBN 0 412 45030 5 1.3.5 Activity 1.3.6 Real SolutionsApart f o any hir dealing for the purposes of research or private study, or rmcriticism o rcviw, as permitted under the UK CopyrigM Dcsigna a d Patents r 1.3.7 Ordered PhasesAct, 1988, this publication may not be reprcduccd,. stoced. or transmitted, in 1.3.8 Intermediate Phasesany form or by any mans, without the prior permission in writing of rhe 1.3 Equilibrium in Heterogeneous Systemspubtishefa, or in thc cast of reprographic reproduction only in accordance with 1.5 Binary Phase Diagramsthe t m of the licencts issued by the Copyright Lictasing Agmcy in the UK,or in accordance with the tams o f li- issued by the appropriate I 3 . 1 A Simple Phase DiagramReproduction Rights Organization outside the U K Enquiries concerning 1.5.2 Systems with a Miscibility Gaprcproduftion outside the t e r m slated hwe should be sglt to the publishers at the 1.5.3 Ordered Alloys London add- printed on this page. 1.5.4 Simple Eutectic Systems The publisher makta no repmentation, expmss or implied, with regard t thc o 1.5.5 Phase Diagrams Containing Intermediate Phasesaccuracy of the information conktined in this book and cannot accept any legal 1.5.6 TheGibbsPhaseRulerwponsibility or liability for any crmrs or omissions that may be made. 1.5.7 The Effect of Temperature on Solid Solubility 1.5.1: Equilibrium Vacancy ConcentrationA Cataiogut m r d for this book is available ftom the British Library 1.6 The Influence of Interfaces on EquilibriumLibrary o f Congreu Cataloging-in-Publication Data available 1.7 Ternary Equilibrium 1.8 Additional Thermodynamic Relationships for Binary Solutions 1.9 The Kinetics of Phase Transformations Referencesn Further ReadingBPrinted on permanent acid-fm text apsr manufa~tuAin accordance with ANSUNIS0 239.48-1992 and ANSUNLO239.4% 1984 (Pcrmansncc of Paper). Exercises
vi Con (enIS Confen~s vii2 Diffusion 3.3.3Second-Phase Shape: Misfit Strain Effects 2.1 Atomic Mechanisms of Diffusion Fully Coherent Precipitates 2.2 Interstitial Diffusion Incoherent Inclusions 2.7.1 Interstitial Diffusion as a Random Jump Process Plate-Like Precipitates 2.2.2 Effect of Temperature-Thermal Activation 2.2.3 Steady-State Diffusion 2.2.4 Nonsteady-State Diffusion _ 3.4.3 Coherency Loss 3.4.5 Glissiie Interfaces 3.1.6 SolidlLiquid Interfaces 2.2.5 Solutions to the Diffusion Equation 3.5 Interface Migration Homogenization 3.5.1 Diffusion-Controlled and Interface-Controlled Growth The Carburization of Steel References 2.3 Substitutional Diffusion Further Reading 2.3.1 Self-Diffusion Exercises 2.3.2 Vacancy Diffusion 2.3.3 Diffusion in Substitutional Allnys 4 Solidification 185 2.3.4 Diffusion in Dilute Substitutional Alloys 4. I Nucleation in Pure Metals 135 2.4 Atomic Mobility 4.1.1 Homo~eneous Nuclealion 18b 2.5 Tracer Diffusion in Binary Alloys 4.1.2 The Homogeneous Nucleot~onRate 190 2.6 Diffusion in Ternary Alloys 4.1.3 Heterogeneous Nucleation 192 2.7 High-Diffusivity Paths 4.1.4 Nucleation of Melting 197 2.7.1 Diffusion along Grain Boundaries end Free Surfaces 4.2 Growth o a Pure Solid f 197 2.7.2 Diffusion along Dislocations 4.2.1 Continuous Growth 198 2.8 Diffusion in Multiphase Binary Svstems 1.2.1 Lateral Growth 198 References Surface Nucleation 1(M Further Reading Sp~ral Growth 20 1 Exercises Growth from Twin Intersections 202 4.2.3 Heat Flow and Interface Stability 2033 Crystal Interfaces and Microstructure 4.3 Alloy Solidification 1117 3.1 Interfacial Free Energy 4.1.1 Solidiiication of Single-Phase Alloys 208 3.2 SolidJVapour Interfaces Equliibrium Solidification 108 3.3 Boundaries in Single-Phase Solids No Diffusion in Solid. Perfect Mixing in Liquid 208 3.3.1 Low-Angle and High-Angle Boundaries No Diffusion in Solid, Diffusional Mixing In tiquld 212 3.3.2 Special High-Angle Grain Boundaries Cellular and Dendritic Solidification 214 3.3.3 Equilibrium in Polycrystalline Materials -4.3.2 Eutectic Solidification 222 3.3.4 Thermally Activated Migration of Grain Boundaries Growth of Lamellar Eutectics 223 3.3.5 The Kinetics of Grain Growth 4.3.3 Off-Eutectic Alloys 229 3.4 Interphase Interfaces in Solids 4.3.1 Perltectic Solidification 73 1 3.3. f Interface Coherence 4.4 Solidification of Ingots and Castings 233 Fully Coherent Interfaces 4.4.1 Ingot Structure 233 Semicoheren t interfaces Chill Zone 234 Incoherent Interfaces Columnar Zone 735 Complex Semicoherent Interfaces Equiaxed Zone 236 3.4.2 Second-Phase Shape: Interfacial Energy Effects Shrinkage Effects 236 . Fully Coherent Precipitates 4.4.2 Segegation in lngots and Castings 237 Partially Coherent Precipitates 4.4.3 Continuous Casting 233 Incoherent Precipitates Heat Flow in Welding and Continuous Precipitates on Grain Boundaries Casting 239
4.5 Solidification of Fusion Welds Upper Bainite Influence of Welding Speed Lower Bainite Geometry of Crystal Growth Transformation Shears 4.6 Solidification during Quenching from the Melt 5.8.3 The Effect of Alloying Elements on Hardenability 4.7 Case Studies of some Practical Castings and Welds 5.8.1 Continuous Cooling Diagrams 4.7.1 Casting of Carbon and Low-Alloy Steels in 5.8.5 Fibrous and Interphase Precipit~tion Alloy Steels - 1.7.2 Casting of High-Speed Steels 5 -9 Massive Transformat ions , 3.7.3 Stainless Steel Weld Metal 5.10 Ordering Transformarions References 5.1 1 Case Studies Further Reading 5.11.1 Titanium Forging Allays Exercises 5.1 1.2 The Weldability of Low-Carhnn and Microalloyed Rolled Steels References5 Diffusional Transformations in Solids Further Reading 5.1 Homogeneous Nucleation in Solids Exercises 5.2 Heterogeneous Nucleation Nucleation on Grain Boundaries 6 Diffusionless Transformations Dislocations h. 1 Characteristics uf Diffusionless Transformilttons Excess Vacancies h. 1 . 1 The Solid Solution of Carbon in Iron 5.2.1 Rate of Heterogeneous Nudeation 2 Martensite Uryatallu~raphy 5.3 Precipitate Growth h.2.1 The Bain Model of the fcc + hct Transformation 5.3.1 Gruwth behind Planar Incoherent Interfaces 6 . 2 . 2 Comparison of Crystallographic Thcory with Sa3.2 Diffusion-Contmlled Lengthening of Plates or Needles Experimental Results -3% 5.3.3 Thickening of Plate-like Precipitates h.3 Theories o f Martensite Nucleation 397 5.1 Overall Transformation Kinetics-TIT Diagrams h.3.1 F(~rmation Coherent Nuclei of Marttssite of 398 -i .S Precipitation in Age-Hardening Alloys 6.3.1 Role of Dislocations in Martunhitc ?iuclculion 101 5.5.1 Precipitation in Aluminium-Copper Alloys h.3.3 Dislocation Strain Energ! A+%is~ed Transformation 10h GP Zones h.4 Martensite Growth 100 Transition Phases 15.4.I Growth of Larh Martensite - 410 5.6.2 Precipitation in Aluminium-Silver Alloys 6.4.2 Plate Martensite 412 5.5.3 Quenched-in Vacancies 6.4.3 Stabilization 415 5.5.4 Age Hardening 6.4.4 . Effect of External Stresses 415 5.5.5 Spinodat Decompositic>n 6.4.5 Role of Grain Size Jlh 3.5.6 Particle Coarsening 6.5 Pre-martensite Phenomena Jlh Low y 6.6 Tempering of Ferrous Martensites 417 Low x, Carbon Segregation 420 Low D E-Carbide 421 -,. 5.6 The Precipitation of Ferrite from Austenite Cementite -122 5.7 Cellular Precipitation AHoy Carbides 412 5.8 Eutectoid Transformations Effect of Retamed Austenite 476 -. 5.8. I The Pearlite Reaction in Fe-C Alloys Recovery, Recrystallization and Grain Growth 42h Nucleation of Pearlite Temper Emhrittlement 127 .. Pearlite Growth 6.7 Case studies 428 Pearlite in Off-Eutectoid Fe-C Alloys 6.7.1 Carbon and Low-Alloy Quenched and Tempered Steels 428 5.8.2 The Bainite Transformation 6.7.2 Controlled Transformation Steels 430
6.7.3 The Shape-Memory Metal: Nitinol References Further Reading ExercisesSolutions to exercisesCompiled by John C. IonIndev * 439 441 I I Preface to the second edition 510 : I n the ten years since this book was tirst published there have been man): new developments in the rnetallureical field. Rapidly solidified metals and glasses have come of age; new AI-Li alloys are now used in modem aircraft; microalloyed (structural) and high purity (pipeline) steels have become more sophisticated: radically new oxide-dispersed steels have ap- peared; a number of new memory metals have been developed: the list could go on. In spite of this. the undertyins principles governing ail of these developments have obviously not changed over the years. This is really the strength of the present text book. From the beginning we aimed to spell out these principles in a nice. readable way, and one in which undergraduates could appreciate and he capahle of developing for themselves. The present text is thus deliberately little changed from the original. We have, however. hopefully .corrected any errors. expanded the lists o f further reading, and perhaps. most importantly. included a complete set of solutions to exercises. We hope that the revised edition continues to be enjoyed and appreciated in the many Schools of Metallur~y, Materials Science and Engineering Materials we know t o he using our text throughout the world. In completing this rcvlsed edition we are grateful to the many people. students and professors ;dike, who have written to us over the last decade. Part~cularthanks are due to Dr Wen-Bin Li (Un~versity Lulei) for using of a fine tooth-comb in bringing out both obvious and less obvious errors in the original text. There remain, (inevitably). a few points of contention concerning ourde~cri~tion certain phenomena. as raised by some of our of correspondents, but there is nothing unhealthy about that. We should finail! like to thank Dr John Ion (University of Lappeenranta, Finland) for his help in compiling the Solutions to Exercises chapter. David Porter and Kenneth Easterling September 1W l
... Xlll ~ r i f u u e rhe firsr edirion ro 1 support and encouragement of our colleagues and students in the Depari- ment of Engineerins Materials. Particular thanks are due LO Agneta Engfors I for her patience and skill in typing the manuscript as well as assisring with I the editingPreface to the first edition David Porter and Kenneth Easterling * Frhruury 1980This book is written as an undergraduate course in phase transformationsfor final year students specializing in metallurgy, materials science orengineering materials. It should also be useful for research students in-terested in revising their knowledge of the subject. The book is based onlectures originally given by the authors at the University of Lulel forengineerins students specializing in engineering materials. Surprisingly wefound no modern treatments of this important subject in a form suitable fora course book, the most recent probably being P.G. Shewmons Tram-formations in Metals (McGraw-Hilt, 1969). There have, however, been somenotable developments in the subject over the last decade, particularly instudies of interfaces between phases and interface migration, as well as thekinetics of precipitate growth and the stability of precipitates. There havealso been a number of important new practical developments based onphase transformations, including the introduction of TRIP steels (trans-formation induced by plastic deformation). directionally aligned eutecticcomposites. and sophisticated new structural steeIs with superior weldabilityand forming properties. to mention just a few. In addition. continuouscasting and high speed, high energy fusion welding have emerged strongly inrecent years as irnportant production applications of solidification. It was theobjective of this course to present a treatment of phase transformations inwhich these and other new developments could be explained in terms of thebasic principles of thermodynamics and atomic mechanisms. The book is effectively in two parts. Chapters 1-3 contain the backgroundmaterial necessary for understanding phase transformations: thermo-dynamics, kinetic-., diffusion theory and the structure and properties ofinterfaces. Chapters 4-6 deal with specific transformations: solidification,diffusional transformations in solids and diffusionless transformations. Atthe end of the chapters on solidification, diffusion-controlled transforma-tions and martensite, we give a few selected case studies of engineeringalloys to illustrate sorne.of the principles discussed earlier. In this way, wehope that the text wil1:provide 9 usefu~ Link between theory and the practicalreality. It should be stated that we found it necessary to give this course inconjunction with a number of practical laboratory exercises and workedexamples. Scts of problems are aIso included at the end of each chapter ofthe book. In developing this course and wriring the text we have had continuous
Thermodynamics and Phase Diagrams- I t This chapter deals with some of the basic thermodynamic concepts that are required for a more fundamental appreciation of phase diagrams and phase transformations. It is assumed that the student is already acquainted with elementary thermodynamics and only a summary of the most important results as regards phase transformations will be given here. Fuller treatment can be found in the books listed in the bibliography at the end of this chapter. The main use of thermodynamics in physical metallurgy is to allow the prediction of whether an alloy is in equilibrium. In considering phase trans- formations we are always concerned with changes towards equiiibrium. and thermodynamics is therefore a very powerful tool. It should be noted. how- ever. that the rate at which equilibrium is reached cannot be determined by thermodynamics alone, as will become apparent in later chapters. 1.1 Equilibrium It is useful to begin this chapter on thermodynamics by defining a few of the terms that will be frequently used. In the study of phase transformations we will be dealing with the changes that can occur within a given system, e.g. an alloy that can exlst as a mixture of one or more phases. A phase can be defined as a portion of the system whose properties and composition are . homogeneous and which is physically distinct from other parts of the system. The components of a given system are the different elements or chemical compounds which make up the system, and the composition of a phase or the system can be described by giving the relative amounts o each component. f The study of phase transformations, as the name suggests, is concerned with how one o r more phases in an alloy (the system) change into a new phase or mixture of phases. The reason why a transformation occurs at all 1s because the initial state of the alloy is unstable relative to the final state. But how is phase stability measured? The answer to this question is provided by thermo- dynamics. For transformations that occur at constant temperature and pres- sure the relative stability of a system is determined by its GIbbs free energy (G). The Gibbs free energy of a system is defined by the equation I w h e k H is the enthslpy, T the absolute temperature, and S the entropy of the i system. Enthalpy is a measure of the heat content of the system and is given i
Thermodynamic-s arid phase diagranls I Equilibriumwhere E is the internal energy of the system. P the pressure, and V thevolume. The internal energy arises from the total kinetic and potential ener-gies of the atoms within the system. Kinetic energy can arise from atomic G~bbsfreevibration in solids or liquids and from translational and rotational energies for energythe atoms and molecules within a liquid or ga$ whereas potential energyarises from the interactions, or bands. between the atoms within the system.If a transformation or reaction occurs the heat that is absorbed o r evolved willdepend on the change in the internaI energy of the system. However it wiilalso depend on changes in the volume of the system and the term P V takesthis into account, so that at consmntpressure the heat absorbed or evolved isgiven by the change in H . When dealing with condensed phases (solids andliquids) the P V term is usually very small in comparison t o E , that is H = E. Arrcngement of atomsThis approximation wiIl be made frequently in the treatments given in this Fig 1.1 .4 schematic r nr~atic-rn f Glbt-rc free ene;g with thc arrangement of ;itom5 obook. The other function rhat appears in the expression for G is entropy (S) Contigurat~on A hiis the lotvest tree energ! and i s thtrufcrrc the ananptmenr when .which is a measure of the randomness of the system. rhe $>stern 1s at stable equilibrium Confipurat~clnB 1s a metastable r q u i l ~ b r ~ u r n . A system is said t o be in equilibrium when it is in the most stable state. i.e.shows n o desire to change ad infinifurn. An important consequence of thelaws of classical thermodynamics is that at constant temperature and pressurea closed system (i.e. one of fixed mass and composition) will be in stableequilibrium if it has the lowest possible value of the Gibbs free energy, or in - uqiiilihriutn states to distlnpujsh them from rhr siuhlc rquilihriiirn state. The intermediate states for which dC; 0 are iinsruhle and are only ever realized rnoment-nrily in pracrice. If. as the result uf thermal fluctuarions, the atomsmathematical terms become arranged in an lnterrnediate state they will rapidly rearrange into one of the free energy minima. [f by a change of temperature or pressurt. for example. a system is moved from a stable to a rnerastablr srarc i t will. g i w n It can be seen from the definition of G, Equation 1.1, that the state with the time. transform to tho new $table equilibrium state. highest stability will be that with the best compromise between low enthalpy Graphite and diamond at ruurn iempersturr and pressure are examples u fand high entropy. Thus at tow temperatures solid phases are most stable since stable and metastable equilibrium states. Given time. therefore. all diamondthey have the strongest atomic binding and therefore the lowest internal under these conditions will transform to graphite.energy (enthalpy). At high temperatures however the - TS term dominates Any transformation that results in a decrease in Gibhs tree energy isand phases with more freedom of atom movement, liquids and gases, become possible. Therefore a necessary criterion for any phase transformation ismost stable. If pressure changes are considered it can be seen. fromEquation 1.2 that phases with smaII volumes are fz---uredby high pressures. The definition of equilibrium given by Equation 1.3 can be illustrated where C;, and G 2 are the free energies of the initla1 and final states respec-graphically as follows. If it were possible to evaluate the free energy of a given tlvely. The transformation need not go directly to the stable equllibriurn statesystem for all conceivable configurations the stable equilibrium configuration but can pass through a whole series of intermediate metastable states.would be found to have the lowest free energy. This is illustrated in Fig. 1.1 The answer to the quest~on "How fast does phase transformation occur?"where it is imagined that the various atomic configurations can be represented is not provided by classical thermodynamics. Sometimes metastable states canby points along the abscissa. Configuration A wouId be the stable equilibriumstate. At this point small changes in the arrangement of atoms to a first be very short-l~ved:at o t h q times they can exist almost indefin~telyas in the case of diamond at roam tirnperature and pressure. The reason for these .+ *approximation produce no change in G, I-e. Equation 1.3 applies. However differences i s the presence of the free e n e r g hump between the metastable .there will always be other configurations, e.g. B, which lie at a tocal minimum and stable states in Fig. 1.1. The study o transformation rates in physical fin free energy and therefore also satisfy Equation 1.3, but which do not havethe lowest possible value of G. Such configurations are called metastable 1 chemistry belongs to the realm of kinetics. In general. higher humps or energy barriers lead to siower transformation rates. Kinetics obviously plays a central I
Therrnodytmmics and phase diagrums Sirtgle compvnenl systemsrole in the study of phase transformations and many examples of kineticprocesses will be found throughout this book. The different thermodynamic functions that have been mentioned in thissection can be divided into two types called intensive and extensive prop-erties. The intensive properties are those which are independent of the size ofthe system such as T and P, whereas the extensive properties are directly Iproportional to the quantity of material in the system. e.g. P, E , H, and G. S IThe usual way of measuring the size of the system is by the number of moles iof material it contains. The extensive properties are then molar quantities, t ,i.e. expressed in units per mole. The number of moles of a given component -in the system is given by the mass of the component in grams divided by its (0)atomic or molecular weight. The number of atoms or molecules within 1 mol of materiaj is given byAvogadros number ( N , ) and is 6.023 X loz3.1.2 Single Component SystemsLet us begin by dealing with the phase changes that can be induced in a singlecomponent by changes in temperature at afxed pressure, say 1 atm. A singlecomponent system could be one containing a pure element or one type of diK)molecule that does not dissociate over the range of temperature of interest. Inorder to predict the phases that are stable or mixtures that are in equilibriumat different temperatures it is necessary to be able to calculate the variation ofG with T .1.2.1 Gibbs Free Energy as a Function of TemperatureThe specific heat of most substances is easily measured and readily available.In general it varies with temperature as shown in Fig. 1.2a. Tfie specific heatis the quantity of heat (in joules) required to raise the t e r y x a t u r e o the f Entropysubstance by one degree Ketvin. At constant pressure this is denoted by C , sand is given by 1 cp= (g) P (1.5) 1 0 T(K)Therefore the variation of H with T can be obtained from a knowledge of the Ic) 0 . ~ i 1.2 (a) Variation of C, with temperature, C,, tends to a h i t of -3R- tb) ~ ,variation of C, with T. In considering phase transformations or chemical Vanation ofenthatpy ( H ) with abolute temperature for a pure metal. (c) Variationreactions it is only changes in thermodynamic functions that are of interest. of entropy ( S ) with absolute temperature.Consequently H can be measured relative t o any reference level which is Iusuallydone by defining H = 0 for a pure element in its most stable state at298 K (25 "C). v9iation of N with T can then be calculated by integrating The
6 Thermodynamics and phase diagramEquation 1.5, i.e.The variation is shown schematically in Fig. I .2b. The slope of the H-Tcurve is Cp. The vanation of entropy with temperature can also be denved from thespecific heat C From classical thermodynamics ,.Taking entropy at zero degrees Kelvin as zero, Equation 1.7 can be inte-grated to giveas shown in Fig. 1 . 2 ~ . Finally the variation of G wirh temperature shown in Fig. 1.3 is obtainedby combining Fig. 1.2b and c using Equation 1.1. When temperature andpressure vary the change in Gibhs free energy can be obtained from thefollowing result of classica1 thermodynamics: for a system o fixed mass fand composition F I ~1.3 . V a r i a t ~ u nuf Gibhs free energ!- wlth temperature dG = -SdT + VdP (1.9)At constant pressure dP = 0 and supplied to the system will not raise its Temperature but will be used in supplying the latent heat of melting ( L ) that is required to convert solid into liquid (bc in Fig. 1.4). Note that at Tm the specific heat appears to be i n h n ~ t e since the addition of heat does not appear as an increase in temperature. When all solid has transformed into liquid the enthalpy of the system willThis means that G decreases with increasing T at a rate given by -3. The follow the line cd while the Gibbs free energy decreases along ef. At srillrelative positions of the free energy curves of solid and liquid phases art higher temperatures than shown in Fig. 1.4 the free energy of the gar vhaseillustrated in Fig. 1.4. At all te..yeratures the liquid has a higher enthalpy (at atmospheric pressure) becomes lower than that of the liquid and the liquid(internal energy) than the solid. Therefore at low temperatures G~ > G ~ . transforms to a gas. If the solid phase can exist in different crystal structuresHowever, the liquid phase has a higher entropy than the solid phase and the (allotropes or polyrnorphs) free energy curves can be constructed for each ofGibbs free energy of the liquid therefore decreases more rapidly with increas- I these phases and the temperature at which they intersect will give the equilib-ing temperature than that of the solid. For temperatures up t o Tm the solidphase has the lowest free energy and is therefore the stable equilibrium 1 : rium temperature for the polymorphic transformation. For example at atmos- pheric pressure iron can exist as either bcc ferrite below 910 "C or fccphase, whereas above T , the liquid phase is the equilibrium state of thesystem. At T , both phases have the same value of G and both solid and liquid ! austenite above 910 "C, and at 910 "C both phases can exist in equilibrium.can exist i equilibrium. T. is therefore the equilibrium melting temprahlre nat the pressure concerned. i ! 1.2.2 Pressure Eflecrs If a pure component is heated from absolute zero the heat supplied willraise the enthalpy at a rate determined by C (solid) along the line ab in ,Fig. 1.4. Meanwhile the free energy wl decrease along ae. At T the heat il , ! : The equilibrium temperatures dircusse~iso far only apply at a specific pres- sure ( 1 a t m , say). At o ~ h e r pre3sures the equilibrium temperatures will differ.
8 Thermodynamics and phnsr diagrums L Y Y - iron Pressure, kbar Fig. 1.5 Effect of pressure on the equilibrium phase diagram for pure iron pressure. The only way to maintain equilibrium at different pressures is bv taryins the temperature. If the two phases in equilibrium are u and P. application of Equation 1.9 to 1 mol of both gives dc" = V",P - SUdT (1.12) dG" V z d P - SPdT solid stablrstoble If a and p are in equilibrium G" = GBtherefore dU" = dGp and IFig. 1.4 Variarion of enthalpy ( H ) and free energy (G) with temperature for thesolid and iiquid phases of a pure metal. L i s the latent heat of melting, Tm the , , .equilibrium melting temperature. This equation gives the change in temperature d T required to maintain e~uilibriumbetseea a and 0 if pressure is increased by d P . The equation can bd s;..jplifiedas follows. From ~ ~ u a t i o n 1.1For example Fig. 1.5 shows the etfect of pressure on the equilibrium tempera-tures for pure iron. Increasing pressure has the effect of depressing the u/y G" = HU - TS"equilibrium temperature and raising the equilibrium melting temperature. At GP = ~ f - TS@ ivery hgh prearures hcp E-Fe becomes stable. The reason for these changesderives from Equation 1.9. At constant temperature the free energy of a Therefore, putting dG = Gp - Ga etc. givesphase increases with pressure such that = AH - TAS ..But since at equilibrium G~ = Ga,G = 0. and (1.13) AH - TAS = 0 If the two phases in equilibrium have different molar volumes their Consequently Equathn 1.13 becomesrespective free energies will not increase by the same amount at a giventemperature and equilibrium will, therefore, be disturbed by changes i n
I0 Therrnocllrlurnics and pflusr diagrunr~ which is known as the Clausius-Clapeyron equation. Since close-packed whers y-Fe has a smaller molar volume than a-Fe. AV = V i - V,",< 0 whereas AH = H - H" > 0 (for the same reason that a liquid has a higher enthalpy than a solid). so that (dP!dTI is negative, i.e. an increase in pressure lowers L ~the t equilibrium melting temperature T , the free energies of solid and the equilibrium transition temperature. On the other hand the 6;L equilib- liquid are equal. i.e. AG = U. Consequently rium temperature is raised with increasing pressure due to the larger molar volume of the liquid phase. It can be seen that the ef€ect of increasing pressure is to increase the area of the phase diagram over which the phase and therefore at T , with the smallest molar volume is stable (y-Fe in Fig. 1.5). It should also be noted that E-Fe has the highest density of the rhree allotropes. consistent with the slopes of the phase boundaries in the Fe phase diagram. This is known as the entropy of fusion. It is observed experimentally that 1.2.3 The Driving Forcrjor Solidification the entropy of fusion is a constant =R(S.3 1 mol- K-) for mart metals (Richards rule). This is not unremonable as metals with high bond strengthsIn dealing with phase transfurmations we are often concerned with the can be expected to have high values for both L and T,,.difference in free energy between two phases at temperatures away from the For small undercoolings ( A T ) the difference in the specific heats of theequilibrium temperature. For example. if a liquid rne~al undercooled by 1 T is liquid and solid (Cb - CP) can be isnored. AH and 15 are therefore approx-below Tm before it solidifies, solidification will be accompanied by a decrease ~rnatel!, independent of temperature. Combining Equations I . 15 and 1.16in frer energy AG (I mol-) as shown in Fig. 1.h. This free energy decrease thus givesprovides the driving force for solidilcatiun. The miignitude of this change canbe obtained as follows. The frer energies of rhe liquid and solid at a lrmperaturr T a r e given by c;~= - ffL TS i.e. for small ATTherefore at a temperature T This i s a very useful result which will frequently recur In subsequent chapters. 1 1.3 Binarv Solutions I In single component systems all phases have the same composition, and equilibrium simply involves pressure and temperature as variables. In alloys. AG however. composition is also variable and tu understand phase changes in alloys requ~res appreciation of how the Gibbs free energy of a given phase an : depends on compositiun as well as temperature and pressure Since the phase . I . transformafions described in this book mainly occur at a fixed pressure of I I G 1 arm most attention will be given to changes in composition and tempera- I ture. In order to introduce some of the basic concepts of the therrnodyndmics Cr-4 6 i of allays a simple physical model for binary solid solutions will be described. i I i L 1 I j 1.3.1 The Gibhs Free Energy of Binary Solutions T Tm ure T m~emt e IFig. 1 6 Difference in free cnsrgr between liquid and The Gibbs free energy of a binary solufion of A and B atoms be ihr point,The curvature of the ad d -lines has heen lgnorcd l calculated from the free energies o f pure A and pure B In the following
12 phuse diugrums Thermodynamiw u~zdIt is assumed that A and B have the same crystal structures in their pure statesand can be mixed in any proportions to make a solid soIution with the samecrystal structure. Imagine that 1 mol of homogeneous solid solution is made Free energyby mixing together XA rnol of A and X , mot of B . Since there is a total of p e r moleI mol of sohtion before mixingand X and XB are the molefrnctiom of A and 3 respectively in the alloy. In , 1I GA 4order to calculate the free energy of the alloy. the mixing can be made in twosteps (see Fig. 1.7). These are: 1 1 f 0 A 1 x, - J 1 0 1. bring together XA rnol of pure A and X, mol of purt! 3 ; 2. allow the A and B atoms to m x together to make a homogeneous solid ; i i of V a r ~ a t l u n G I (the free cnrrgy hefore mixing) wirh alloy composit~on1.y.4 solution. iAfter step 1 the free energy of the system i s given by hr. expresqcd as ( 1.20) G: = GI -where C, and GB are the molar free energes of pure A and pure B at the uhere LG.,,, i s the change In Ghbs frte energy caused hy the m~xine.temperature and pressure of the above experiment. GI can be most conve- ,niently represented on a molar free energy diagram (Fig. 1.8) in which molarfree energy is plotted as a function of Xg or XA, all alloy compositions GI For 1Ilies on the straight line between GA and GB. L The free energy of the system will not remain constant during the mixing of andthe A and I atoms and after step 2 the free energy of the solid solution G , can 3 C :; = HI - TS1 ? putting Before m i x i n g After mixing i i 1 and MIX IS",,,S - s, = : w AH,,, is the heat absorbed or evolved during step 2. i . c it is the heat of X4 molA .EE. XA GA XBmol B EE. XB GB .. - 1 mol salid solution - .+ I 5oiution, and ignoring v ~ l u m echanges during the process, it represents only the difference in internal energy ( E )before and after mixing. AS,,, is the difference in cntgopj: fietween the mixed and unmixed states: . Total free energy= Toto 1 free energy = I 1.3.2 Ideal Soiurions GI = X A G A + X ~ G * G2 G Fig. 1.7 Free energy o mixing. f r + AGmlx I The simplest type of miring to treat first is when AH,,, = 0. in which case the resultant solution i said tn be ideal and the free energy change on mixing is s
14 T~~ermad~nnrnirs phase diagrams und Binary solurionsonly due to the change in entropy: In statistical thermodynamics, entropy is quantitatively related to random-ness by the Boltzmann equation. i.e. S = kLno (12 3 )where k is Boltzmanns constant and w is a measure of randomness. There aretwo contributions to the entropy of a solid solution-a thermal contributionS,, and a configurational contribution S,,,,, . In the case of thermal entropy, w is the number of ways in which thethermal energy of the solid can be divided among the atoms. that is, the total 6number of ways in which vibrations can be set up in the solid. In solutions.additional randomness exists due to the different ways in which the atoms can i A Fig. 1.9 Free energy of mixing for an ideal solution.be arranged. This gives extra entropy ScOnfi,o which w is the number of frdistinguishable ways of arranging the atoms in the solution. If there is n o volume change or heat change during mixing then t h e onlycontribution to AS,,, is the change in configurational entropy. Before mixing, This is shown schematically in Fig. 1.10. Note that. as the temperaturethe A and B atoms are held separately in the system and there is only one increases. GA and GA decrease and the free energy curves assume a greaterdistinguishable way in which the atoms can be arranged. Consequently curvature. The decrease in G,,, and GB is due to the thermal entropy of bothS, = kln 1 = 0 and therefore AS,,, = 5:. components and is given by Equation 1.10. Assuming that A and B mix to form a substitutional solid solution and that It should be noted that all of the free energy-composition diagrams in thisall configurations of A and 3 atoms are equally probable, the number of book are essentially schematic; if properly plotted the free energy curvesdistinguishable ways of arranging the atoms on the atom sites is must end asymptot~cally at the verticai axes of the pure components. i.e. tanyentlal to the vertical axes of the diagrams. This can be shnwn by differentiating Equation 1.26 or 1.27.where N, is the number of A atoms and .YB the number of B atoms. Since we are dealing with 1 mu1 of solution, i.e, rV, atoms (Avogadrosnumber). Molar free energyand A, = X B N , V - By substituting into Equations 1.23 and 1.24, using Stirlings approxima-tion (In N! N ln - N ) and the relationship N,k = R (the universal gasconstant) gives A,, S, = - R ( X A In X + X, ln XB) , (1.25)Note that. since XA and X, are less than unity, AS,,, is positive. 1.e. there isan increase in entropy on mixing, as expected. The free energy of mixing,AC,,,, is obtained from Equation 1.22 as I . A,, G, = R T ( X , In XA + XB In XB) (1.26) , 0 4 3Figure 1.9 shows AG,,, as a function of composition and temperature. " + - !,/fC(~~-5q,k> - ! % I The actual free energy of the solution G will also depend on G , and G,. Fig. 1.10 The molar free energy (free energy per mole of solution) for an deal solidFrom Equations 1.19. 1.20 and 1.26 d t i t i o n 4 ct,mhination of Fig<. I H :ltld 1.9.
lh Thermoiiyrlamics and phuse diagrams1.3.3 Chemical PotentialIn alloys it is of interest to know how the free e n q y of a given phase willchange when atoms are added or removed. If a small quantity of A, dn, mol,is added to a large amount of a phase at constant temperature and pressure,the size of the system wiIl increase by dn, and therefore the rota1 free energyof the system will also increase by a small amount dG. If dnA is small enoughdG will be proportional to the amount of A added. Thus we can write dC = pAdnA (T, P, n~ constant) (1.28)The proportionality constant p, is called the partial molar free energy of A oralternatively the chemical potential of A in the phase. FA depends on the Fig 1 . 1 1 The relationship between the trcc energy curve tor a rolutton and thecomposition of the phase, and therefore dn, must be so small that thecomposition is not significantly altered. If Equation 1.28 is rewritten it can beseen that a definition of the chemical potential of A is chemical potent~alsof the components. sides of the molar free energ!. d~ngramas shown in Fig. 1.1 1. This can be - obtained from Equations 1 .?ii and 1 3 1 . remembering that X,4 + XB = I . i.c. dxA= -dXB. and this is left as an erercist for ihe reader. I t i clear from , Fig. 1 . 1 l that p A and pR vary systemnticillly with ihr cumposition of theThe symbol G has been used for the Gibbs free energy to emphasize the fact phase.that it refers to the whole system. The usual symbol G will be used to denote Comparison of Equation, 1.17 and 1.31 gi?er I.L, and p~ for an idealthe molar free energy and is therefore independent of the size of the system. solution as Equations similar to 1.28 and 1.29 can be written for the other components k, = G , + R T i n X,*in the solution. For a binary soIution at constant temperature and pressurethe separate contributions can be summed: FB = - G B R T l n XB xhich is a much simpler wa! of presrnring Equation 1.17. These relationships are shown in Fig. 1.11. Thr. distances ac and bd are simply - R T In ., and YThis equation can be extended by adding further terms for solutions contain- -RT In X , .ing more than two components. If T and P changes are also allowedEquation 1.9 must be added giving the general equationIf 1 mol of the original phase contained X, mol A and XB mol B, the size ofthe system can be increased without altering its composition if A and B areadded in the correct proportions, i.e. such that dn,: dnB = X, : X . For ,example if the phase contains twice as many A as B atoms(X, = 2 / 3 , X, = 1/31 the composition can be maintained constant byadding two A atoms for every one B atom (dn,: dnB = 2). In this way thesize of the system can be increased by 1 mol without. changing p and p g .TO ,.do this XAmo1 A and X m01 B must be added and the free energy o the g fsystem will increase by the molar free energy G. Therefore fromEquation 1.30 When G is known as a function of X and X,, as in Fig. 1.10 for example, ,p and FB can be obtained by extrapolating the tangent to the G curve to the , A I XB - 1 6 FIF. 1.17 The relationship beween the free energy curve and chzmlcal potentlais for an ideal solution.
18 Therrnod~~namics p h a s ~ und diugrums Binarv solutions1.3.4 Regular SolutionsReturning to the model of a solid soiution, so far it has been assumed thatAH,,, = 0; however, this type of behaviour is exceptional in practice andusually mixing is endorhermic (heat absorbed) or exothermic (heat evolved).The simple model used for an ideal solution can, however, be extended toinclude the AH,,, term b,- using the so-called quasi-chemicalapproach. that is. E is the difference between the A-B bond energy and the average o f In the quasi-chemical model it is assumed that the heat of mixing, AHmi,,is the A-A and B-B bond energies.only due to the bond energies between adjacent atoms. For this assumption t o If E = 0. AHmix 0 and the solution is ideal. as considered i = nbe valid it is necessary that the volumes of pure A and 3 are equal and do not Section 1.3.2. In this case the atoms are completely randomly arranged andchange during mixing so that the interatomic distances and bond energies are the entropy of m x n is given by Equation 1.25. In such a solution it can also iigindependent of composition. be shown1 that The structure of a binary solid solution is shown schematically in Fig. 1.13. (1.35)Three tvpes of interatomic bonds are present: i PAB= Na:XAXB bonds mol- I i 1. A-A bonds each with an energy,,E . where N, 1s Avogadros aumber, and i IS the number of bonds per atom. 2. B-B bonds each with, an energy E B B , i If E < 0 the atoms in the solution will prefer to be surrounded by atoms of 3 . A-B bonds each with an energy E, . : the opposite type and this will increase P A Dwhereas, if E > 0. P,4Bwill tend . to be less than in a random solution. However, provided E is not too differentBy considering zero energy to be the state where the atoms are separated to from zero, Equation 1.35 is still a good approximation in which caseinfinity E A , ~ .E B B and E A R are negative quantities. and become increasingly (1.36)more negative as the bonds become stronger. The internal energy of the AH,,, = ItX,XBsolution E will depend on the number of bonds of-each type P A , , P,, and 1 whereP,4B such that fl = ;Y,zE 1 Reai solutions that closely obe! Equation 1.35 are known as regular soh-Before mixing pure A and B contain only A-A and B-B bonds respec- , rions. The variation of AH,,, with composition is parabolic and is shown intively and by considering the relationships between PA,. P,, and P A , in the i Fig, 1.14 for R > 0. Pjote that the fangents at XA = 0 and 1 are related to 0solution i t can be shown1 that the change in internal energy on mixing is given as shown. AHmix per mol I Fig, 1-14 The of AH,,, with composition for a regular solution.
20 Thermodynamics und phase dil~grarns Binury solutions 21 The free energy change on mixing a regular solution is given by value 12 (Fig. 1.14). This means that, except at absolute zero, AG,, alwaysEquations 1.21, 1.25 and 1.36 as decreases o n addition of a small amount of solute. The actual free energy of the al:oy depends on the values chosen for C, and GB and is given bv Equations 1.19, 1.20 and 1.38 as G = XAGA 7 XBGB W 4 X B + R T ( X , I XA + XB In XB) (1.39) + nfisir shown i Fig. 1.15 for different values of d and temperature. For n ! This ir shown in Fig. 1.16 along with the chemical potentials of A and B in theexothermic solutions AHmi,< 0 and mixing results in a free energy decrease sotution. Using the relationship XAXB= X x + X a A and comparingat all temperatures (Fig. 1.15a and b). When AH,,, > 0, however, the situa- Equarions 1.31 and 1.39 shows that for a regular solutiontion is more complicated. At high temperatures TAS,* i s greater than AHH,,for all compositions and the free energy curve has a positive curvature at qA = G A 4 fl(1 + - xAI2 RT ln X,all points (Fig. 1.15~). low temperatures, on the other hand, TAS,, is At andsmaller and hGmi,develops a negative curvature in the middle (Fig. 1.15d). Differentiating Equation 1.25 shows that, as XA or XB-+ 0, the - TAS,, p, = GB A fl(1 - x~)+ RT In XBcurve becomes vertical whereas the slope of the AH,,, curve tends to a finite Expression 1.32 for the chemical potential of an ideal alloy was simple and it is convenient to retain a similar expression for any solutioi~. This can be done by defining the a c t i v i ~ a component. a. such that the distances ac and bd in of Fig. 1.16 are - R T I a, and -RT In a ~ In. this case n pA = GA + RT ln a , ~ and I I I A AGmix 8 A B (a) R<O,highT (b) n-= 0 , I o w T A w B A B (c) n > o , high T (d), n> o IOW T Fig. 1.15 The effect o AH,,,,, T on hGmi,. f and Fig. 1.16 The relationship between molar free energy and activity
-- 1 and phase diagram ~trrrnouynamzcs 1 Binary solutiorrs 23 Ih general a and a, will be different from X, and XB anct the relationstup , Equation 1.44 is known as Henrys law and 1.45 as Raoults law; they apply tobetween them will vary with the composition of the solution. For a regular solutions when sufficiently dilute.solution, comparison of Equations 1.40 and 1.11 gives Since activity is simply related to chemical potential via Equation 1.41 the activity of a component is just another means of describing the state of the component in a solution. NO extra information is supplied and its use is simply a matter of convenience as it often leads to simpler mathematics.and Activity and chemical potential are simply a measure of the tendency of an atom to leave a solutiirn. If the activity or chemical potential is low the atoms are reluctant to leave the solution which means, for example, that the vapour pressure of the component in equilibrium with rhe soiution will be relativelyAssuming pure A and pure B have the same crystal structure, the rela- low. It will also be apparent later that the activity or chemical potential of ationship between a and X for any solution can be represented graphically component is important when several condensed phases are in equilibrium.as illustrated in Fig. 1.17. Line 1 represents an ideal soIution for whicha, = X, and a~ = XB. AHmix < 0 the activity of the components in Ifsolution will be less in an ideal solution (line 2) and vice versa when AH,, 1.3.6 Real Solutions> 0 (line 3). he ratio (aA/XA)is usually referred to as y,, the activity cdefficient of A, Ii While the previous model provides a useful description of the effects ofthat is I configurational entropy and interatomic bonding on the free energy of binary solutions its practical use is rather limited. For many systems the model is an For a dilute solution of B in A, Equation 1.32 can be simplified by letting oversimplification of reality and does not predict the correct dependence ofXB-+ 0 in which case : AG,,, on composirton and temperature. UB As already indicated, in alloys where the enthalpy of mixing is not zero Y B = = constant (Henrys law) . (1.44) i I (E and fl # 0) the assumption that a randurrl arrangement of atoms is the XB equilibrium. or most stable arrangement is not true. and the calculated valueand for A,, will not give the minimum free energy. The actual arrangement of G, QA atoms will be a compromise that gives the lowest internal energy consistent 1 (Raoults law) (1.45) with sufficient entropy. or randomness, to achieve the minimum free energy. In systems with E < 0 the internal energy of the system is reduced by increas- ing the number of A-B bonds, i.e. by ordering the atoms as shown in Fig. 1.18a. If E > 0 the internal energy can be reduced by increasing the number of A-A and B-B bonds, i.e. by the clustering of the atoms into A-rich and B-rich groups, Fig. 1.18b. However, the degree of ordering or (a) (b) (c> Fig. 1.18 Schematic representation o f , soiid solutions: (a) ordered substitutional, (b} clustering, (c) random interstitial.
24 Thermudynornrcs und phme diagrams i Binary sol1rtions 15 clustering will decrease as temperature increases due to the increasing impor- tance of entropy. In systems where there is a size difference between the atoms the quasi- chemical model will underestimate the change in internal energy on mixing since no account is taken of the elastic strain fields which introduce a strain energy term into AH,,,,,. When rhe size difference is large this effect can dominate over the chemical term. When the size difference between the atoms is very large then inrersnriai solid solutions are energetically most favourable, F ~ E1 . 1 8 ~New mathemati- . . (al (b) cal models are needed to describe these solutions. Fie, 1.19 (a) Random A - B solution with a total of 100 atoms and X A = = 1 1 5. In sysrems where there is strong chemical bonding between the atoms there p - - 1 ) S = U. (b) Same allo!. with short-range order PAfi= .:;1 is a tendency for the formation of intermetallic phases. These are distinct from solutions based on the pure components since they have a different crystal structure and may also be highly ordered. Intermediate phases and I ! p,~, - 100. S = (132 - 10(3)/(100 - 100) 0.37. point as shown in Fig. 1.20a. At low temperatures, however. solutions with ordered phases are discussed further in the next twn sections. - _- - - -- 2 1 Xc-, = XAu= 0.j. i.e. a 50/50 C u i A u mixture, form an ordered structure in which the Cu and Au atoms are arranged in alternate layers. Fig. 1 .?Ob. Each t atom position is no lonser equivalent and the lattice is described as i1 CuAu -- .. .- . 1.3.7 Ordered Phases , ,,-L, - . : siiperlatrice. i n alloys with the composition Cu3Au another superlattice is found. Fig. 1.20~. If the atoms in a substitutional solid solution are completely randomly The entropy of mixing of structures with long-range order is extremely small and with increasing temperature the degree of nrder decreases until. arranged each atom position is equivalent and the probability that any given site in the lattice will contain an A atom will he equal to the fraction of A i above some critical temperature there is no Inng-range order at all. This atoms in the solution X , similarly XBfor the B atoms. In such solutions PAR, i temperature is a maximum when the composition is the ideal required for the , the number of A-B bonds, is given by Equation 1.35. If R < O and the : superlattice. However. long-range order can still be obtained when the com- number of A-B bonds is greater than this, the solution is said to contain position deviates from the ideal if sume of the atom sites are left vacant or if shorr-range order (SRO). The degree of ordering can be quantified bv de- some atoms sit on wrong sites. I n such cases i t can be easier to disrupt the fining a SRO parameter s such that - order with increasing temperature and thc critical temperature is lower. see Fis. 1.21. a The most common ordered lattices in other systems are summarized in i Fig. 1.72 along with their Structurbericilr notation and examples of alloys in i which they are found. Finally, note that the critical temperature for loss of l o ~ n g order i n c i e a m i n c r e a r i n p 0. or I H , , , . a i s ! e m s where P,,(max) and P,,(random) refer to the maximum number of bonds 1 e possible and the number of bonds for a random solution, respectively. Figure 1.19 illustrates the difference between random and short-range ordered solutions. ixudzd -- - phase is stable un to the meliing point. In solutions with compositions that are close to a simple ratio of A : B atoms another Type of order can be found as shown schematically in Fig. 1.l8a. This is known as long-range order. Now the atom sites are no longer equivalent but cm be labelled as A-sites and B-sites. !Such a solution can be considered to be a different (ordered) phase separate from the random or nearly random solution. Consider Cu-Au alloys as a specific example. Cu and Au are both fcc and ~ C OAUO C U U orAu totally miscible. At high temperatures Cu or Au atoms can occupy any site Fig. l.M Ordered subs~itutionaltructurcs In the Cu-Au rystcm: ( a ) high-tempera- and the lattice can be considered as fcc with a random atom at each lattice rure disordered structure. ( b l UuAu superlatt~ce.( c ) CulAu cuperlattice.